# Mechanical Properties of Metals How do metals respond to external ```Chapter Outline
Mechanical Properties of Metals
How do metals respond to external loads?
 Stress and Strain
&frac34; Tension
&frac34; Compression
&frac34; Shear
&frac34; Torsion
 Elastic deformation
 Plastic Deformation
&frac34; Yield Strength
&frac34; Tensile Strength
&frac34; Ductility
&frac34; Toughness
&frac34; Hardness
Optional reading (not tested): details of the different types
of hardness tests, variability of material properties
(starting from the middle of page 174)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
1
Introduction
Stress, σ (MPa)
To understand and describe how materials deform
(elongate, compress, twist) or break as a function of
applied load, time, temperature, and other conditions we
need first to discuss standard test methods and standard
language for mechanical properties of materials.
Strain, ε (mm / mm)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
2
Tensile
Compressive
Shear
Torsion
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
3
Concepts of Stress and Strain
(tension and compression)
To compare specimens of different sizes, the load is
calculated per unit area.
Engineering stress:
σ = F / Ao
F is load applied perpendicular to speciment crosssection; A0 is cross-sectional area (perpendicular to
the force) before application of the load.
Engineering strain:
ε = Δl / lo (&times; 100 %)
Δl is change in length, lo is the original length.
These definitions of stress and strain allow one to
compare test results for specimens of different crosssectional area A0 and of different length l0.
Stress and strain are positive for tensile loads, negative
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
4
Concepts of Stress and Strain
(shear and torsion)
Shear stress:
τ = F / Ao
F is load applied parallel to the upper and lower faces
each of which has an area A0.
γ = tgθ (&times; 100 %)
Shear strain:
θ is strain angle
Torsion is variation of pure shear. The shear stress in
this case is a function of applied torque T, shear strain
is related to the angle of twist, φ.
Shear
Torsion
Ao
F
θ
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
5
Stress-Strain Behavior
Elastic Plastic
Elastic deformation
Reversible: when the stress
is removed, the material
returns to the dimensions it
Stress
Usually strains are small
(except for the case of some
plastics, e.g. rubber).
Plastic deformation
Irreversible: when the stress
is removed, the material
dimensions.
Strain
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
6
Stress-Strain Behavior: Elastic Deformation
In tensile tests, if the deformation is elastic, the stressstrain relationship is called Hooke's law:
σ = Eε
E is Young's modulus or modulus of elasticity, has the
same units as σ, N/m2 or Pa
Stress
Slope = modulus of
elasticity E
Strain
Higher E → higher “stiffness”
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
7
Elastic Deformation: Nonlinear Elastic Behavior
In some materials (many polymers, concrete...), elastic
deformation is not linear, but it is still reversible.
Δσ/Δε = tangent modulus at σ2
Definitions of E
Δσ/Δε = secant modulus
between origin and σ1
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
8
Chapter 2:
force-separation
curve for
interacting atoms
Energy, eV, Force, eV/&Aring;
Elastic Deformation: Atomic scale picture
0.005
Force
0
Energy
-0.005
-0.01
2
4
6
8
Distance between atoms, rij, &Aring;
E ~ (dF/dr) at ro
(r0 – equilibrium separation)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
9
Elastic Deformation: Anelasticity
(time dependence of elastic deformation)
• So far we have assumed that elastic deformation is
time independent (i.e. applied stress produces
instantaneous elastic strain)
• However, in reality elastic deformation takes time
(finite rate of atomic/molecular deformation
load release. This time dependent elastic behavior
is known as anelasticity.
• The effect is normally small for metals but can be
significant for polymers (“visco-elastic behavior”).
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
10
Elastic Deformation: Poisson’s ratio
εy
εx
ν=− =−
εz
εz
Materials subject to tension shrink laterally. Those
subject to compression, bulge. The ratio of lateral and
the above equations shows that lateral strain is in
opposite sense to longitudinal strain
υ is dimensionless
Theoretical value for isotropic material: 0.25
Maximum value: 0.50, Typical value: 0.24 - 0.30
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
11
Elastic Deformation: Shear Modulus
Δy
Zo
τ
Relationship of shear stress to shear strain:
τ = G γ, where: γ = tgθ = Δy / zo
G is Shear Modulus (Units: N/m2 or Pa)
For isotropic material:
E = 2G(1+υ) → G ~ 0.4E
(Note: single crystals are usually elastically
anisotropic: the elastic behavior varies with
crystallographic direction, see Chapter 3)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
12
engineering stress
Stress-Strain Behavior: Plastic deformation
engineering strain
Plastic deformation:
&frac34; stress and strain are not proportional to each other
&frac34; the deformation is not reversible
&frac34; deformation occurs by breaking and re-arrangement of
atomic bonds (in crystalline materials primarily by
motion of dislocations, Chapter 7)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
13
Tensile Properties: Yielding
Elastic Plastic
Stress
σy
Yield strength σy - is chosen as
that causing a permanent strain
of 0.002
Yield point P - the strain deviates
from being proportional to the stress
(the proportional limit)
The yield stress is a measure of
resistance to plastic deformation
Strain
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
14
Tensile Properties: Yielding
Stress
Strain
In some materials (e.g. low-carbon steel), the stress
vs. strain curve includes two yield points (upper and
lower). The yield strength is defined in this case as
the average stress at the lower yield point.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
15
Tensile Strength
If stress = tensile strength is maintained
then specimen will eventually break
Stress, σ
fracture
strength
“Necking”
Tensile strength: maximum
stress (~ 100 - 1000 MPa)
Strain, ε
For structural applications, the yield stress is usually a
more important property than the tensile strength, since
once the yield stress has passed, the structure has deformed
beyond acceptable limits.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
16
Tensile properties: Ductility
Lo
Ao
Af
Lf
Ductility is a measure of the deformation at fracture
⎛ lf − l0 ⎞
⎟⎟ &times; 100
Defined by percent elongation %EL = ⎜⎜
⎝ l0 ⎠
(plastic tensile strain at failure)
or percent reduction in area
MSE 2090: Introduction to Materials Science
⎛ A0 − Af
%RA = ⎜⎜
⎝ A0
⎞
⎟⎟ &times; 100
⎠
Chapter 6, Mechanical Properties
17
Typical mechanical properties of metals
The yield strength and tensile strength vary with prior
thermal and mechanical treatment, impurity levels,
etc. This variability is related to the behavior of
dislocations in the material, Chapter 7. But elastic
moduli are relatively insensitive to these effects.
The yield and tensile strengths and modulus of
elasticity decrease with increasing temperature,
ductility increases with temperature.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
18
Toughness
Toughness = the ability to absorb energy up to
fracture = the total area under the strain-stress
curve up to fracture
εf
∫ σdε
0
Units: the energy per unit volume, e.g. J/m3
Can be measured by an impact test (Chapter 8).
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
19
True Stress and Strain
True stress = load divided by
actual area in the necked-down
region (Ai):
σ = F/A
T
i
Sometimes it is convenient to use
true strain defined as
εT = ln(li/lo)
True stress continues to rise to the point of fracture, in
contrast to the engineering stress.
σT = F/Ai εT = ln(li/lo)
If no volume change
occurs during deformation,
Aili = A0l0 and the true and
engineering stress and
stress are related as
σ = F/Ao ε = (li-lo/lo)
σT = σ(1 + ε)
εT = ln(1 + ε)
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
20
Elastic Recovery During Plastic Deformation
If a material is deformed plastically and the stress is then
released, the material ends up with a permanent strain.
If the stress is reapplied, the material again responds
elastically at the beginning up to a new yield point that is
higher than the original yield point.
The amount of elastic strain that it will take before
reaching the yield point is called elastic strain recovery.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
21
Hardness (I)
Hardness is a measure of the material’s resistance
to localized plastic deformation (e.g. dent or scratch)
A qualitative Moh’s scale, determined by the ability of
a material to scratch another material: from 1 (softest
= talc) to 10 (hardest = diamond).
Different types of quantitative
hardness test has been designed
(Rockwell, Brinell, Vickers, etc.).
Usually a small indenter (sphere,
cone, or pyramid) is forced into the
surface of a material under
conditions of controlled magnitude
size of indentation is measured.
The tests somewhat approximate,
but popular because they are easy
and non-destructive (except for the
small dent).
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
22
Tensile strength (MPa)
Tensile strength (103 psi)
Hardness (II)
Brinell hardness number
Both tensile strength and hardness may be regarded as
degree of resistance to plastic deformation.
Hardness is proportional to the tensile strength - but
note that the proportionality constant is different for
different materials.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
23
Stress
What are the limits of “safe” deformation?
For practical engineering design,
the yield strength is usually the
important parameter
Strain
Design stress: σd = N’σc where σc = maximum
anticipated stress, N’ is the “design factor” &gt; 1. Want to
make sure that σd &lt; σy
Safe or working stress: σw = σy/N where N is “factor of
safety” &gt; 1.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
24
Summary
&frac34; Stress and strain: Size-independent measures of load
and displacement, respectively.
&frac34; Elastic behavior: Reversible mechanical deformation,
often shows a linear relation between stress and strain.
&frac34; Elastic deformation is characterized by elastic moduli
(E or G). To minimize deformation, select a material
with a large elastic moduli (E or G).
&frac34; Plastic behavior: Permanent deformation, occurs
when the tensile (or compressive) uniaxial stress
reaches the yield strength σy.
&frac34; Tensile strength: maximum stress supported by the
material.
&frac34; Toughness: The energy needed to break a unit
volume of material.
&frac34; Ductility: The plastic strain at failure.
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
25
Summary
Make sure you understand language and concepts:
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
&frac34;
Anelasticity
Ductility
Elastic deformation
Elastic recovery
Engineering strain and stress
Engineering stress
Hardness
Modulus of elasticity
Plastic deformation
Poisson’s ratio
Shear
Tensile strength
True strain and stress
Toughness
Yielding
Yield strength
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
26
Chapter 7: Dislocations and Strengthening Mechanisms
&frac34;
Dislocations and Plastic Deformation
9 Motion of dislocations in response to stress
9 Slip Systems
9 Plastic deformation in
 single crystals
 polycrystalline materials
&frac34; Strengthening mechanisms
9 Grain Size Reduction
9 Solid Solution Strengthening
9 Strain Hardening
&frac34; Recovery, Recrystallization, and Grain Growth
Optional reading (Part that is not covered / not tested):
7.7 Deformation by twinning
In our discussion of slip systems, &sect;7.4, we will not get into
direction and plane nomenclature
MSE 2090: Introduction to Materials Science
Chapter 6, Mechanical Properties
27
```